# New Methods for Evaluation of Spent Fuel Condition during Long-Term Storage in Slovakia

Authors: M. Mikloš; V. Kršjak
Journal: Science and Technology of Nuclear Installations
 (2009)

---

## Abstract

Experiences with an advanced spent nuclear fuel management in Slovakia are presented in this paper. The evaluation and monitoring procedures are based on practices at the Slovak wet interim spent fuel storage facility in NPP Jaslovské Bohunice. Since 1999, leak testing of WWER-440 fuel assemblies are provided by special leak tightness detection system “Sipping in pool” delivered by Framatomeanp with external heating for the precise defects determination. In 2006, a new inspection stand “SVYP-440” for monitoring of spent nuclear fuel condition was inserted. This stand has the possibility to open WWER-440 fuel assemblies and examine fuel elements. Optimal ways of spent fuel disposal and monitoring of nuclear fuel condition were designed. With appropriate approach of conservativeness, new factor for specifying spent fuel leak tightness is introduced in the paper. By using computer simulations (based on SCALE 4.4a code) for fission products creation and measurements by system “Sipping in pool,” the limit values of leak tightness were established.


---

## Body

## 1. Introduction

The Interim Spent Fuel Storage Facility (ISFSF) in Jaslovské Bohunice [1–3] is an important component of the spent nuclear fuel management system. The facility has been used for storage purposes since 1987. ISFSF is a nuclear facility providing for a safe storage of the spent nuclear fuel from VVER-440 reactors for the time period of 50 years before the fuel is further processed in a reprocessing plant or appropriately disposed off.It is necessary to keep the concentration of fission products in storage pools on the low level for assurance of acceptable activity of the coolant. This can be done with periodical monitoring of the fuel elements condition, defects identification, and closing of leaking assemblies or fuel elements, respectively, in special hermetic caskets. This was the main reason for including not only “Sipping in pool” system, but also inspection stand “SVYP-440” (Figure1), into the ISFSF operation [4–7].Equipment for VVER-440 spent fuel assemblies control in Slovakia.
(a)
Sipping in pool(b)
SVYP-440The system “Sipping in pool” was built and implemented in the storage facility operation in 1999 and since then, the important results have been measured. The system increases the temperature of the fuel assembly (by external heaters), which cause the increasing of the pressure inside fuel elements. If there is any leakage, increased pressure will cause higher fission product release. By measurement of released activity, the assembly tightness is determined.Since December 2006, the new stand for VVER-440 fuel assemblies’ inspection “SVYP-440” is in operation. By using several modules, it has ability to open and take the fuel assembly apart, so it can examine all fuel elements. If the defect is found, fuel element with defect is closed into the special hermetic case.


## 2. Experimental

Slovakia has more than 20 years of experience with spent fuel storage. Since beginning, there were no leakages detected during storage conditions. Even though the negative effects of fuel cladding are very low, however, due to degradation of Zirconium alloys after long periods of under water storage, there is a finite possibility of defect formation. It is also difficult to estimate the long-term degradation process. With use of the systems like “Sipping in Pool” or “SVYP-440,” the leakages of the fuel assembly can be detected.In that case, it is necessary to have as conservative approach to the extent possible. If we compare the volume activity of released fission products around fuel assemblyAO (measured by “Sipping in Pool”) and the volume activity of fission products inside whole fuel assembly AI (calculated by SCALE code), we could estimate the fuel cladding condition. Therefore, we are introducing the fuel cladding leak tightness  coefficientkFCT:(1)kFCT=AOAI.For the calculations of volume activity of fission products (in particular,137Cs has been considered) inside whole fuel assembly, sequence ORIGEN-ARP have been used (for version SCALE 4.4a) [8, 9]. As a simplification of the calculations, one model of fuel assembly has been used for all measured assemblies. This model, created by VUJE, a.s. company (Ing. Vladimír Chrapčiak, Ing. Radoslav Zajac, December 2002), is a standard model of VVER-440 fuel assembly, with the UOX fuel and 4.2% enrichment of 235U. Only burnup, power, effective days during operation and days during shut downs were unique for every assembly.


## 3. Results

After SCALE calculations of volume activity of137Cs inside the fuel assemblies, and measurements of volume activity of 137Cs outside the fuel assemblies by “Sipping in Pool,” 36 values of the fuel cladding leak tightness coefficients kFCT have been obtained (Table 1). All values were described by distribution function (Figure 2) to determine the mean value μ and standard deviation σ. It means that all fuel assemblies with kFCT = 1.1·10-10±6.5·10-11, or (μ+1·σ), are without any leakages. Fuel assemblies’ producer criteria for the released γ activity of fission products are 10-4 Ci/L (3.7·106 Bq/L). Because there were only small differences (less the 101) between the measured summary gama activity and the separated cesium activity, we compared these two activities.Table 1
Measured and calculated values ofAO and AI and final calculation of kFCT.
Number of FAAO [Bq/L]AO [Bq]AI to 1 kgU [Ci]AI to 1 FA [Bq]kFCT163963 90082.73.678E+141.73736E-10260960 90082.73.678E+141.65579E-10352752 7001155.11451E+141.0304E-10456356 3001135.02556E+141.12027E-10553553 5001135.02556E+141.06456E-10660960 9001185.24793E+141.16046E-10742142 10086.43.84255E+141.09563E-10858458 40081.33.61574E+141.61516E-10948348 3001024.53635E+141.06473E-101053953 90086.43.84255E+141.40271E-101148448 40080.83.5935E+141.34688E-101253653 60080.83.5935E+141.49158E-101362762 7001004.4474E+141.40981E-1014135 00013500 0001034.58082E+142.94707E-08156740674 0001094.84767E+141.39036E-091674 0007400 0001094.84767E+141.52651E-081737237 200793.51345E+141.05879E-101836636 600793.51345E+141.04171E-101927727 7001225.42583E+145.10521E-112044144 1001225.42583E+148.12779E-112146146 1001255.55925E+148.29249E-112228828 8001325.87057E+144.90583E-112343743 70077.73.45563E+141.2646E-102431031 00077.73.45563E+148.97087E-112550550 5001114.93661E+141.02297E-102634634 6001114.93661E+147.00885E-112785485 4001145.07004E+141.68441E-102823823 8001145.07004E+144.69425E-112932032 00075.63.36223E+149.51748E-113018218 20075.63.36223E+145.41307E-113127827 8001265.60372E+144.96099E-113215015 0001185.24793E+142.85827E-113336636 6001195.29241E+146.91557E-113410510 5001245.51478E+141.90398E-11352030203 00074.53.31331E+146.1268E-10363880388 00074.53.31331E+141.17103E-09Figure 2
Distribution function of continuous variablekFCT.Figure 3
Limit values for the fuel cladding leak tightness coefficientkFCT.There were two limit values calculated:(a)
kFCT=3·10-10,(b)
kFCT=8·10-7.The first value,kFCT=1.1·10-10±1.95·10-10=3·10-10, or (μ+3·σ) is from the statistical dispersion of distribution function of continuous kFCT, and means that 99.73% of the values are within 3 standard deviation. In other words, kFCT=3·10-10 means that with the probability of 99.73% will be all measured and calculated assemblies tight.The second value is calculated with use of fuel assemblies’ producer criteriaAOP=3.7·106 Bq/L(2)kFCT=AOAI=3.7·108Bq4.4655·1014Bq=8.06·10-7,whereAO=AOP*Vs, Vs: volume of the Sipping casket [3, 4], and AI: average value of the calculated AI (Table 1).By considering by this value, we set the final limit intervals:(1)
(0-3·10-10):values of the fuel cladding leak tightness coefficient for tight fuel assembly— kFCT(T),(2)
(3·10-10-8·10-7):values of the fuel cladding leak tightness coefficient for fuel assembly suspicious from leakage— kFCT (SL),(3)
(8·10-7-1):values of the fuel cladding leak tightness coefficient for fuel assembly with leakage—kFCT (L).The optimal use of the cladding leak tightness coefficientkFCT is its application during periodical monitoring of fuel assemblies. Because of the low level of summary γ activity in the coolant, monitoring of 6 fuel assemblies at ISFSF in Jaslovské Bohunice is provided once per year. Two assemblies are marked as reference, other 4 assemblies are chosen randomly. For those two reference assemblies, values of the cladding leak tightness coefficient kFCT were calculated. For both assemblies (Figures 4 and 5), the values of kFCT are about 1.2·10-10. Only during last measurement, few deviations have been observed. The deviation for first assembly is +7.73·σ, and for second assembly it is +16.3·σ. This means, that both fuel assemblies are susceptible to the leak tightness. However, during measurements in 2007, values of kFCT increased for every measured assembly. So, the “jumps” can be caused by incorrect measurements by “Sipping in Pool.”Figure 4
Values ofkFCT for reference FA number 1.Figure 5
Values ofkFCT for reference FA number 2.


## 4. Conclusions

From the nuclear safety point of view, it is necessary to keep the fission products inside the fuel elements and to prevent their escape into environment not only during reactor operation or fuel transport, but also during the long-term storage of spent nuclear fuel. Therefore, the effective leak tightness monitoring system at all fuel interim storages is necessary. The designed system from the 80s at the Slovak wet interim storage facility did not assure this task at the desired level, so the system “Sipping in Pool” was implemented in 1999. After several years of its operation, performed measurements showed that this system is highly effective equipment for fuel cladding defects detection. Since 2006 a new inspection stand “SVYP-440” for monitoring of spent nuclear fuel condition is used as well.New factor for specifying of spent fuel leak tightness has been introduced. Using the computer simulations (based on SCALE 4.4a code) for fission products creation and measurements by the system “Sipping in Pool,” the limit values of the cladding leak tightness coefficientkFCT has been defined. It is a tool, which is used as additional information, describing fuel cladding leak tightness criteria. Forward-looking, the authors expect that the mean value of kFCT will oscillate about 10-10. Contingent deviations could be caused by incorrect measurements by “Sipping in Pool,” or using of incorrect fuel assembly model for SCALE calculations. Also, the leak tightness coefficient kFCT will depend on the pool water cleaning system. Depending on the residual activity in the pool, the values of kFCT will change. Therefore, further research is needed.



---

*Source: 459139-2009-10-13.xml*